# The Influence of Solid State Diffusion - Lehigh University Influence of Solid State Diffusion ......

date post

19-Apr-2018Category

## Documents

view

212download

0

Embed Size (px)

### Transcript of The Influence of Solid State Diffusion - Lehigh University Influence of Solid State Diffusion ......

The Influence of Solid State Diffusion on Microstructural Development During Solidification

J.N. DuPont

Department of Materials Science and Engineering

Lehigh University, Bethlehem, PA 18015 jnd1@lehigh.edu

Keywords: Solidification, solid state diffusion, microstructural development

Abstract. The primary factors that effect solid state diffusion during solidification are described and

binary solute redistribution equations that permit estimation of the significance of solid state

diffusion are discussed. Model calculations suggest that solid state diffusion of substitutional

alloying elements in FCC alloys is insignificant under most processing conditions, while that of

interstitial alloying elements is likely to be complete. Experimental data that supports these results

are presented. Several cases that highlight the practical importance of microsegregation on

performance of engineering alloys are described as well as methods for avoiding or minimizing

microsegregation for improved properties. A solute redistribution model for handling the limiting

cases of solute diffusion in ternary alloys is presented and model calculations are reviewed to reveal

the strong influence diffusion can have on the solidification path and resultant microstructure.

Introduction

Solidification processing is used in a variety of fabrication methods such as casting, welding, laser

surface treatment, and crystal growth. In many cases, products prepared from these processes are

utilized in the as-solidified condition. In such applications, the mechanical properties and corrosion

performance of the component are strongly influenced by the distribution of alloying elements and

relative fraction of secondary constituents which form during the solidification process. It is often

useful to make quantitative estimates of the resultant solidification microstructure as a means for

controlling the ultimate component performance. The degree of solid state diffusion that occurs

during solidification plays an important role in microstructural development. The objective of this

article is to review factors that influence the extent of solid state diffusion that occurs during

solidification, describe methods for estimating the expected degree of solid state diffusion, and

discuss various models that can be used to account for the influence of solid state diffusion on the

solidification path and resultant phase formation. Pertinent solute redistribution models for binary

and ternary alloys will be described, and practical examples that highlight the importance of solid

state diffusion will be provided.

Limiting Cases of Solute Redistribution in Binary Alloys

Many models have been developed in the solidification literature on solute redistribution and

microstructural development in binary alloys that are capable of accounting for factors such as solid

state diffusion, dendrite tip undercooling, and coarsening, and several review articles have been

published on the subject [1-4]. While these models are quite useful, it is worth noting that most all

conditions of solute redistribution in binary alloys must fall within two very simple cases: the lever

law and so-called non-equilibrium Scheil equation [5]. Each of these conditions assumes that

equilibrium is maintained at the solid/liquid interface, there is complete diffusion in the liquid, and

there is no undercooling during nucleation or growth. The only difference between the two

conditions is the assumption made about solid state diffusion the lever law assumes solute

diffusion is infinitely fast in the solid while the Scheil equation assumes diffusion is negligible. The

relation between liquid composition and fraction liquid for equilibrium solidification is given

simply by

0

5

10

15

20

25

0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1

fraction liquid

Liquid Composition, wt % B

Equilibrium

Non-Equilibrium

Co = 2 wt% B

a

Fig. 1. Calculated variation in liquid composition during

solidification under equilibrium and non-equilibrium conditions

for a 2 wt% B alloy.

k k)f-(1

C C

L

oL += (1)

where CL is the liquid composition at any value of fraction liquid, fL, Co is the nominal alloy

composition, and k is the equilibrium distribution coefficient, defined as the ratio of solid to liquid

compositions and assumed constant in Eq. 1. The corresponding relation between CL and fL for the

Scheil condition is given by

)1(

LoL fC C= k (2)

These two limiting cases of solute redistribution in binary alloys are quite useful as they

allow the possible ranges of microstructural development to be easily bound. As an example, Fig. 1

shows the variation in liquid composition during solidification under equilibrium and non-

equilibrium conditions for a 2 wt% B alloy from a binary eutectic system that exhibits linear solidus

and liquidus lines, a k value of 0.2, and a eutectic composition of 20 wt% B. The solidification

conditions and resultant microstructure under each extreme are quite different. Under equilibrium

conditions, the liquid composition never becomes enriched to the eutectic composition because

solute in the solid is uniformly distributed and therefore capable of dissolving all the solute before

the eutectic point is reached in the liquid. Note from Eq. 1 that the maximum solute enrichment in

the liquid for the equilibrium condition is given as Co/k, which occurs when fL = 0. In this case, Co/k

< Ce (the eutectic composition). The

resultant microstructure directly after

solidification would simply consist of

primary with a uniform distribution of B. For the non-equilibrium case,

Eq. 2 suggests that CL as fL 0 (for k < 1), which indicates the liquid

composition will always become

enriched to the eutectic point. This can

be attributed to the lack of diffusion in

the primary phase, which leads to the inability of all the solute to be

incorporated into the primary phase.

Thus, directly below the eutectic

temperature, the 2 wt% B alloy

exhibits primary with a concentration gradient and 0.06 weight

fraction of the / eutectic when solidified under non-equilibrium

conditions.

Estimating the Significance of Solid State Diffusion

Although the expressions described above are quite useful, they provide no insight into the possible

role of solid state diffusion for a given solidification condition. Various solute redistribution

equations have been developed over the years that account for solid state diffusion and can be used

to estimate the significance of diffusion. Brody and Flemings [6] were the first to consider the

influence of solid state diffusion on solute redistribution during solidification and, for the case of a

linear growth rate, developed the following expression

1

11

+

=k

sos

k

fkCC

(3)

Where Cs is the solid composition and fs is the fraction solid. The parameter in Eq. 3 is a dimensionless diffusion parameter defined as

2L

tD fs= (4)

Where Ds is the diffusivity of

solute in the solid, tf is the solidification

time (time between the liquidus and

terminal solidus), and L is half the

dendrite arm spacing. The Dstf term in the

numerator essentially represents the

distance the solute can diffuse in the solid

during solidification, while the half

dendrite arm spacing, L, represents the

length of the concentration gradient. Thus,

when Dstf

A

TDs=4

for n = (7a)

3/1

4

A

TDs= for n = (7b)

Eqs. 7 indicate that Ds and T should have the strongest influence on solid state diffusion. Of these, Ds is the most important because it can change by orders of magnitude depending on

temperature, host crystal structure, and the diffusion mechanism. Eqs. 7 also indicate that the

cooling rate should have little or no effect on solid state diffusion during solidification. This can be

understood by considering the competing effects the cooling rate has on the solidification time and

dendrite arm spacing. Lower cooling rates will permit more time for back diffusion (Eq. 5), but the

required diffusion distance also increases since the dendrite arm spacing increases (Eq. 6). These

two opposing effects tend to offset each other so that there is often no significant effect from

cooling rate. Experimental evidence is available to support this. Fig. 2 shows a summary of nominal

and dendrite core measurements acquired on fusion weld made on a Mo bearing stainless steel with

a Mo rich filler metal at various dilution levels [7]. These welds were solidified with cooling rates

of ~ 300 oC/sec. The dendrite core compositions of several samples extracted from the fusion zone

and re-solidified by differential thermal analysis (DTA) at 0.3 oC/sec are also shown. It is interesting

to note that the core compositions are equivalent between samples solidified with cooling rates that

differ by three orders of magnitude, providing verification that cooling rate has a negligible effect

on the back diffusion potential under a wide range of cooling rates for this alloy system.

Recommended

*View more*